Download presentation

1
**Aggregate Properties HMA**

This lecture will discuss those aggregate properties that are associated specifically with HMA. NCAT

2
**To be Covered Specific Gravities Consensus Properties NCAT**

The lecture will discuss aggregate specific gravities and the consensus properties. NCAT

3
**Volumetrics All matter has mass and occupies space.**

Volumetrics are the relationships between mass and volume Superpave mix design based on aggregate and mixture volumetrics NCAT

4
**Specific Gravity, G Mass Solid Volume Mass Water Volume**

Ratio of the mass to volume of an object to that of water at the same temperature Mass Solid Volume Mass Water Volume NCAT

5
**Densities gw = 1.000 g/cm3 gw = 62.4 lb/ft3 gw = 1000 kg/m3**

Density is the unit weight of a material lb/ft3 or kg/m3 Unit weight = g w G gw = g/cm3 gw = 62.4 lb/ft3 gw = 1000 kg/m3 Density is the specific gravity times the unit weight (mass) of water and relates mass to volume: for example, grams per cubic centimeter. Since the unit weight of water in units of 1 g/cm3, this term is sometimes left out of equations shown in test methods. Care needs to be taken if the units of the test are changed. Bulk density means sample contains more than one mass and/or volume NCAT

6
**Bulk Specific Gravity, Dry Vol. of water-perm. voids**

Mass, oven dry Surface Voids Gsb = Vol of agg, + surface voids Vol. of water-perm. voids This slide defines the mass and the volume used to calculate the bulk specific gravity (dry) of aggregates. G designates specific gravity. The subscripts indicate the material tested (s = stone) and the type of specific gravity (b=bulk). In this case, bulk is used because there is more than one component in the volume. NCAT

7
**Bulk Specific Gravity, SSD Vol. of water-perm. voids**

Mass, oven dry agg + mass water Gs, ssd = Vol of agg, + surface voids Vol. of water-perm. voids This slide shows the mass and volumes used to determine the bulk specific gravity, ssd (saturated surface dry). Surface Voids NCAT

8
**Bulk Specific Gravity, Apparent**

This slide shows the mass and volume used to determine the apparent specific gravity. Mass, oven dry agg Gsa = Vol of agg NCAT

9
**Phase: a change in state (e.g. solid, liquid, gas)**

Phase Diagram Phase: a change in state (e.g. solid, liquid, gas) V = (mass) / (Gs gw) Mass (Weight) Volume Water permeable voids A phase diagram is usually used to represent relationships between mass and volume. The specific gravity of each component in the mixture is needed in order to determine the corresponding volume a given mass occupies Aggregate Solids NCAT

10
**Specific Gravity Tests for Aggregates**

Two tests are needed Coarse aggregate (retained on the 4.75 mm sieve) Fine aggregate (passing the 4.75 mm sieve) The specific gravities of aggregates need to be determined separately for the fine and coarse fractions of either a stockpile or a blended material. NCAT

11
**Coarse Aggregate Specific Gravity**

ASTM C127 Dry aggregate Soak in water for 24 hours Decant water Use pre-dampened towel to get SSD condition Determine mass of SSD aggregate in bucket Determine mass under water Dry to constant mass Determine oven dry mass This slide lists the general steps needed to determine the specific gravities of coarse aggregates. NCAT

12
**Coarse Aggregate Specific Gravity**

This photograph shows a sample of aggregate soaking (ready to test), a towel for drying, a spray bottle for pre-wetting the towel, the wire basket for obtaining the weight of SSD aggregate under water, and the water tank under the scale platform. NCAT

13
**Coarse Aggregate Specific Gravity**

The sample of coarse aggregate is being dried. Note the area of aggregate not being worked is covered with the towel so it will not dry out. NCAT

14
**Coarse Aggregate Specific Gravity Calculations**

Gsb = A / (B - C) A = mass oven dry B = mass SSD C = mass under water Gs,SSD = B / (B - C) Gsa = A / (A - C) Water absorption capacity, % Absorption % = [(B - A) / A] * 100 These are the equations for calculating the bulk specific gravity (Gsb), bulk specific gravity saturated surface dry (Gs, SSD), apparent specific gravity (Gsa), and water absorption capacity. The denominator in all of the specific gravity equations is the mass of water displaced by the sample. Since 1 gram of water equals 1 cubic centimeter, this value also represents the volume of water displaced by the sample. NCAT

15
**Fine Aggregate Specific Gravity**

ASTM C128 Dry aggregate Soak in water for 24 hours Spread out and dry to SSD Add 500 g of SSD aggregate to pycnometer of known volume Pre-filled with some water Add more water and agitate until air bubble have been removed Fill to line and determine the mass of the pycnometer, aggregate and water Empty aggregate into pan and dry to constant mass Determine oven dry mass These are the steps necessary for determining the specific gravity of the fine aggregate. NCAT

16
**Fine Aggregate Specific Gravity**

A presoaked sample of fine aggregate is dried back to saturated surface dry condition using a gently moving warm current of air. In this case, a standard hair dryer is used. Saturated surface dry is determined using the cone test. An area is cleared in the center of the work area and the cone is filled to overflowing with the aggregate. The aggregate is then tamped down. NCAT

17
**Fine Aggregate Specific Gravity**

The aggregate is considered to be saturated surface dry when the sand cone slumps when the brass form is removed. NCAT

18
**Fine Aggregate Specific Gravity**

Once the saturated surface dry condition has been achieved, a 500 gram sample (weighed) is placed in a partially filled volumetric glass flask of known volume. The sample is then agitated until the foam and air bubbles have subsided. The flask is then filled with water up to the volumetric mark used for calibration and the mass of the pycnometer (flask), aggregate, and water recorded. NCAT

19
**Fine Aggregate Specific Gravity Calculations**

Gsb = A / (B + S - C) A = mass oven dry B = mass of pycnometer filled with water C = mass pycnometer, SSD aggregate and water S = mass SSD aggregate Gs,SSD = S / (B + S - C) Gsa = A / (B + A - C) Water absorption capacity, % Absorption % = [(S - A) / A] * 100 These equations are similar to those used to determine the specific gravities of the coarse aggregate. Again, the denominator represents the volume of water displaced by the aggregate NCAT

20
**Concensus Aggregate Properties**

Coarse Aggregate Particle Shape % Crushed Faces Flat and Elongated Fine Aggregate Particle Shape Clay Content The consensus aggregate properties of the combined gradation need to be determined once a gradation, or several trial gradations, have been selected. ** Determined for the blended aggregate gradation ** NCAT

21
**Percent Crushed Fragments in Gravels**

Quarried materials always 100% crushed Minimum values depended upon traffic level and layer (lift) Defined as % mass with one or more fractured faces The appropriate percentages of each aggregate stockpile are combined and then split on the 4.75 mm screen. The material retained on the 4.75 mm screen are used to determine the percent crushed faces NCAT

22
**Percent Crushed Fragments in Gravels**

0% Crushed % with 2 or More Crushed Faces This is a measurement of coarse aggregate angularity. The amount of crushing (angularity) is important because it determines the level of internal shear resistance which can be developed in the aggregate structure. Round, uncrushed aggregates tend to “roll” out from under traffic loads and therefore have a low rutting resistance. NCAT

23
**Coarse Aggregate Angularity Criteria**

Traffic Depth from Surface Millions of ESALs < 100 mm > 100 mm < 0.3 < 1 < 3 < 10 < 30 < 100 100 55/-- 65/-- 75/-- 85/80 95/90 100/100 --/-- 50/-- 60/-- 80/75 Superpave requirements are based on both the traffic level and the depth of the layer below the surface. The crushing requirements for low traffic volumes are low or none, regardless of depth. As traffic levels increase, so do the required percentages of crushed faces. There is a higher level of crushing required in the upper 100 mm of the pavement because this is the region which is subjected to the highest shear due to traffic loads. Higher shear forces require a higher level of resistance to shear. First number denotes % with one or more fractured faces Second number denotes % with two or more fractured faces NCAT

24
**Flat and Elongated Particles**

ASTM D4791 Flat Elongated Total flat and elongated Superpave Flat and Elongated Maximum to minimum dimension 5:1 3:1 2:1 Flat and elongated particles are undesirable since they have a tendency to break during construction and under traffic. If they do not break, they tend to produce mixtures with directionally-oriented material properties. NCAT

25
**Flat and Elongated Minimum Maximum NCAT**

The longest dimension of an aggregate particle is used to set one end of the caliber. (pin is at the 5:1 ratio pivot point). NCAT

26
**Flat and Elongated Minimum Maximum NCAT**

The aggregate particle is removed without moving the caliper arm and the narrowest dimension is inserted into the other end. If the aggregate can be inserted without moving the arm, then the particle is flat and elongated at a 5:1 ratio. NCAT

27
**Flat and Elongated Criteria**

Traffic Maximum, Percent Millions of ESALs < 0.3 < 1 < 3 < 10 < 30 < 100 100 -- 10 Currently, the 5:1 ratio is used for Superpave requirements. However, research is being conducted to determine if the 3:1 ratio would be a better parameter. A higher percentage is being considered if the ratio is reduced. NCAT

28
**Fine Aggregate Angularity**

(Uncompacted Void Content of Fine Aggregate) * Fine aggregate at a specified gradation is allowed to flow freely into a 100 cm3 cylinder. *Knowing the specific gravity of the aggregate, the voids between aggregate particles can be determined * The more angular the aggregate, the higher the void content This test is used to ensure a high degree of internal friction in the fine aggregate fractions. Values below about 45 indict more rounded shapes associated with natural sands. NCAT

29
**Fine Aggregate Angularity**

Natural sands: typically < 45 Manufactured sands: typically > 42 The equipment is an inverted mason jar with the bottom cut out and fitted with a conical orifice. A 100 mm3 cylinder is placed below the orifice. One holds a finger over the orifice and charges the jar with the aggregate sample. The aggregate is then allowed to fill the cylinder. Excess aggregate is struck off of the top and the mass of the aggregate needed to fill the known volume is determined. The void content between the aggregate particles is determined using the known volume, the mass of dry aggregate needed to fill the volume, and the bulk specific gravity of the aggregate. NCAT

30
**Fine Aggregate Angularity Criteria**

Traffic Depth from Surface Millions of ESALs < 100 mm > 100mm < 0.3 < 1 < 3 < 10 < 30 < 100 100 -- 40 45 As with the coarse aggregate angularity, the fine aggregate angularity requirements are selected for a given traffic level and depth below the surface. NCAT

31
**Flocculating Solution**

Clay Content (Sand Equivalent Test) * ASHTO T176, ASTM D2419 - Used to estimate the relative proportions of fine agg. and clay-like or plastic fines and dust. SE = Sand Reading Clay Reading *100 Sand Reading Clay Reading Flocculating Solution Suspended Clay Sedimented Aggregate This test estimates the percentage of clay-sized material contained in the fine aggregate fraction. A sample of known volume of fine aggregate is mixed with a flocculating solution in a graduated cylinder and shaken to get the fine material suspended in the solution. The cylinder is allowed to sit for 20 minutes and the height of the material suspended in the solution is determined. The height of the clean aggregate is also determined. The sand equivalent (or clay content) value is reported as the ratio (times 100) of the height of the sand (clean aggregate) to the height of the material in suspension. Note, if there is no clay material, the height of the clay reading equals that of the sand. This gives a sand equivalent value of 100 percent. NCAT

32
**Bottle of Solution on Shelf Above Top of Cylinder**

Hose and Irrigation Tube . Measurement Rod NCAT

33
**Top of Suspended Material**

Marker on Measurement Rod Top of Suspended Material Top of Sand Layer NCAT

34
**Clay Content Criteria 100 Traffic Sand Equivalent**

Millions of ESALs Minimum, Percent < 0.3 < 1 < 3 < 10 < 30 < 100 100 40 45 50 The requirement changes with depth. NCAT

35
Questions - ? NCAT

Similar presentations

Presentation is loading. Please wait....

OK

Aggregate Properties HMA

Aggregate Properties HMA

© 2018 SlidePlayer.com Inc.

All rights reserved.

To ensure the functioning of the site, we use **cookies**. We share information about your activities on the site with our partners and Google partners: social networks and companies engaged in advertising and web analytics. For more information, see the Privacy Policy and Google Privacy & Terms.
Your consent to our cookies if you continue to use this website.

Ads by Google

Ppt on classical economics school Download ppt on world population day Marketing mix ppt on nokia x Download ppt on endangered species in india Detail ppt on filariasis ppt Ppt on statistics for class 11th Ppt on save our planet earth Ppt on adding and subtracting matrices Mis ppt on nokia phone Ppt on tungsten inert gas welding